Enhanced Intercalation Dynamics and Stability of Engineered Micro/Nano-Structured Electrode Materials: Vanadium Oxide Mesocrystals
Post on 09-Dec-2016
Embed Size (px)
The development and implementation of nanostructured materials has led to great enhancements in Li-ion battery performance, as with many other fi elds. [ 1 ] The nanoscale size
Enhanced Intercalation DynaEngineered Micro/Nano-StruVanadium Oxide Mesocrysta
for interfacial Faradaic reactions and the fl ux of Li + across the electrode-electrolyte interface; these effects ultimately enhance the mass and charge diffusion paths and modify the thermodynamics (compared to the bulk), which facilitates phase transitions. [ 2 , 3 ] Provided all the benefi ts of nanostruc-
confi rmed by means of selected area electron diffraction and electron microscopy. It is proposed that the mesocrystal formation mechanism proceeds through classical as well as non-classical crystallization processes, and is possibly facilitated or promoted by the presence of a reducing/chelating agent. The synthesized VO 2 (B) mesocrystals are tested as a cathodic electrode material for lithium-ion batteries, and show good capacity at discharge rates ranging from 1501500 mA g 1 and a cyclic stability of 195 mA h g 1 over fi fty cycles. The superb electrochemical performance of the VO 2 (B) mesocrystals is attributed to the porous and oriented superstructure that ensures large surface area for redox reaction and short diffusion distances. The mesocrystalline structure ensures that all the surfaces are in intimate contact with the electrolyte, and that lithium-ion intercalation occurs uniformly throughout the entire electrode. The exposed (100) facets also lead to fast lithium intercalation, and the homoepitaxial stacking of nanosheets offers a strong inner-sheet binding force that leads to better accommodation of the strain induced during cycling, thus circumventing the capacity fading issues typically associated with VO 2 (B) electrodes. reduction leads to enhancements in the Li-ion battery inter-calation capability by increasing the specifi c surface area
turing, the synthesis and characterization of nanostructured electrode materials of various chemistries have been exten-sively investigated. However, the use of nanostructures is not a panacea, and there are several performance issues, either lingering or deriving from nanostructuring, that still need to be addressed. [ 4 ] Most notably, nanostructured elec-trodes suffer from diminished conductivity, stability, and packing density, while at the same time exhibiting enhanced reactivity. [ 510 ]
The design of structurally aligned nanoparticles can cir-
E. Uchaker, N. Zhou, Y. Li, G. Z. CaoDepartment of Materials Science & EngineeringUniversity of WashingtonSeattle, WA 98195, USAE-mail: email@example.com
M. Gu, C. M. WangEnvironmental Molecular Science LaboratoryPacifi c Northwest National Laboratory Evan Uchaker , Meng Gu , Nan Zhou , Yanwe
An additive and template free process is dmesocrystals via the solvothermal reactioThe six-armed star architectures are compooriented along the  crystallographic 2013 Wiley-VCH Verlag Gm
902 Battelle Boulevard, Richland, WA 99352, USA
small 2013, DOI: 10.1002/smll.201203187mics and Stability of ctured Electrode Materials: ls
i Li , Chongmin Wang , and Guozhong Cao *
eveloped for the facile synthesis of VO 2 (B) n of oxalic acid and vanadium pentoxide. sed of stacked nanosheets homoepitaxially register with respect to one another, as
Mesocrystals1bH & Co. KGaA, Weinheim wileyonlinelibrary.com
cumvent the thermodynamic instability, undesired side reac-tions, high processing costs, and potential nano-toxicity effects associated with nanoparticle synthesis and processing. [ 1 , 11 , 12 ]
E. Uchaker et al.full papersThere has been a great deal of recent efforts in the formation and understanding of ordered nanoparticle superstructures with a vast range of architectures; in particular, crystallo-graphically oriented nanoparticle superstructures, or meso-crystals, have been the central focus of such intrigue since described by Clfen and Antonietti. [ 1316 ] Until recently, meso crystals were only studied in biomineral materials, but current research efforts have shifted towards the devel-opment of mesocrystalline organic molecules, [ 15 , 17 ] metal oxides, [ 1821 ] and other functional materials. [ 22 , 23 ]
Novel nanoparticle arrangement has historically been achieved through the synthesis of nanocrystalline superlat-tices, or supercrystals, and colloidal crystals. However, indi-vidual nanoparticle orientation is not taken into account
Figure 1 . SEM images of the synthesized vanadium oxide mesocrystalsnanosheets composing each arm, d) longitudinal view of star-structure,density. 2 www.small-journal.com 2013 Wiley-VCH
by such assemblies. Mesocrystals can be classifi ed by their high degree of crystallinity, porosity, and subunit alignment along a crystallographic register. [ 14 ] These highly desir-able properties are due in part to the mesocrystal forma-tion mechanisms, which are still poorly understood, and make mesocrystals ideal material candidates for catalysis, sensing, and energy storage/conversion applications. [ 16 ] Mesocrystal growth often proceeds via the aggregation of precursor units, rather than the classical ion-by-ion growth mechanism, which can be attributed with the generation of crystals with hierarchical structures and complex morpholo-gies. Several investigations of mesocrystalline LiFePO 4 and TiO 2 used as the electro-active material for lithium-ion bat-tery electrodes have already been produced, but a report of mesocrystalline vanadium oxide for such an application is lacking. [ 20 , 21 ] Herein, we report on the solvothermal syn-thesis, potential formation mechanism, and electrochemical performance of VO 2 (B) mesocrystals synthesized using an additive free solvothermal approach. Moreover, remarkable phase stability and excellent lithium-ion intercalation prop-erties have been demonstrated for the obtained VO 2 (B) mesocrystals. 2. Results and Discussion
VO 2 (B) mesocrystals were synthesized by adopting the methods of Li et al., which involved the solvothermal reac-tion of V 2 O 5 and oxalic acid.
[ 24 ] The size and morphology of the as-prepared material was examined using scanning elec-tron microscopy (SEM), the results of which are displayed in Figure 1 . Figure 1 ac displays several representative individual mesocrystal assemblies, while Figure 1 df shows an overall SEM micrograph of a typical specimen which is largely composed of uniformly micro-sized ellipsoidal star structures with an average height and width of approximately 2.8 m and 1.5 m, respectively. As the higher magnifi cation images reveal, each star-structure is composed of six arms
: ac) representative view of individual assemblies showing the stacked and e,f) overall view of as-synthesized specimen displaying the packing Verlag GmbH & Co. KGaA, Weinheim
that are self-assembled from stacked nanosheets 2060 nm thick that are radially aligned with respect to the center of the structure. Each nanosheet is intimately connected to its neighbors, resulting in a highly porous structure that should facilitate the penetration of electrolyte into the material, alle-viate cycling induced strain, and decrease the lithium-ion dif-fusion distance. The overall thickness of each hierarchically nanostructured arm is approximately 200300 nm.
Figure 1 e,f illustrates that the star-assemblies appear to have a relatively mono-dispersed size distribution and are tightly packed, which should result in a porous and layered microstructured assembly with enhanced volumetric density and conductivity. A slight degree of variation with the mor-phology is apparent (Figure 1 e); however, such effects are considered negligible because the arms of the structures are composed of stacked nanosheets.
Figure 2 a displays the X-ray diffraction (XRD) pattern of the as synthesized material which can be indexed to the monoclinic crystalline phase of VO 2 (B) (space group C2/m and JCPDS card no. 0812392) with lattice parameters a , b , c , and equal to 12.092 , 3.702 , 6.433 , and 106.6 , respec-tively; this analysis is consistent with literature reports. [ 25 , 26 ]
small 2013, DOI: 10.1002/smll.201203187
Intercalation Dynamics and Stability of Electrode Materials
The interlayer spacing of the phase is determined to be 6.15 from the (001) refl ection. The sharp and high inten-sity diffraction peaks are indicative that the product is highly crystalline. No secondary or parasitic phases are detected, and the formation of crystalline VO 2 (B) indicates that the V 5 + ions from the original V 2 O 5 precursor have been reduced to V 4 + during the solvothermal synthesis by oxalic acid. [ 24 , 27 , 28 ]
Peak broadening analysis of the (001) XRD refl ec-tion using the Scherrer equation indicated that the average crystallite size was approximately 17 nm, substantiating
to be 28.4 m 2 g 1 , which is a reasonable value given the overall microscale of the synthesized assemblies. The amply-sized pores can provide excellent channels and cavities for complete and homogeneous Li + diffusion and intercalation throughout the material. Some residual chelating agent synthesized during the reaction may remain on or between the surfaces of the VO 2 (B) nanosheets, and similar incorpo-rations have been known to decrease the overall porosity of mesocrystals. [ 29 ]
Transmission electron microscopy (TEM) was then performed on a single star-assembly cross section that was pre-
pared using an ultramicrotome, as displayed in Figure 3 a. The cross sectioned image reveals that each arm of the star-assembly is separate from the others, indicating that the structure is not truly single crystalline. Figure 3 b presents the vertex of two arms, as identifi ed by the highlighted region in Figure 3 a, and confi rms the superstructure arms are composed of stacked nanosheets. A thinner ultramicrotomed specimen would have made the nanosheet stacking more pronounced; however, specimens cut to thicknesses of 60 and 80 nm con-tinually shifted when exposed to the electron gun, most
Figure 2 . a) XRD spectrum and the b) BJH desorption pore size distribution for the as synthesized VO 2 (B) mesocrystals (inset: N 2 adsorptiondesorption isotherm). the microscopy results that the VO 2 (B) mesocrystals were composed of nanocrystalline subunits. The presence of the nanoparticle subunits and the porous nature of the sample were confi rmed by the corresponding nitrogen sorption isotherms and BarrettJoynerHalenda (BJH) desorption analyses, which indicated that the majority of pores within the sample are below 15 nm (Figure 2 b). The Brunauer-Emmett-Teller (BET) derived surface area was determined 2013 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Figure 3 . a) TEM image of a cross-sectioned VO 2 (B) star-assembly; b) magnifi ed image of arm int(on the (002) zone axis); d) magnifi ed arm edge; e) overall and f) magnifi ed view showing thcollected 4 h into the solvothermal growth process.
small 2013, DOI: 10.1002/smll.201203187ersection; c) corresponding indexed SAED pattern e  growth direction of the VO 2 (B) nanobelts likely due to heating effects with the epoxy resin (or residual organic matter existing between the nanosheets) when cut so thin. The nanosheets measure several tens of nanometers as observed with TEM, supporting the SEM and XRD fi ndings of the mesocrystalline primary nanoparticle size.
Selected-area electron diffraction (SAED) can be used to demonstrate the single crystalline behavior of mesocrystals due to the subunit nanoparticle alignment 3www.small-journal.com
E. Uchaker et al.
Although the exact formation mechanism is not entirely clear, a schematic of the mesocrystal formation mechanism is proposed and illustrated in Figure 4 , and supported with time resolved SEM growth images (Figure S3, Supporting Infor-mation). Figure 4 a starts off with the VO 2 (B) nanobelts that were directly observed 4 h into the solvothermal treatment. The nanobelts in solution will coarsen and grow into ellip-soidal VO 2 (B) nanosheets through Ostwald ripening. The  growth direction of the VO 2 (B) nanobelts is maintained during this step, as determined from SAED. [ 24 , 28 , 32 ]
Several nanosheets then stack homoepitaxially over one another in order to minimize the energy of the system. Residual chelating agent remaining on the (100) surface of each nanosheet effectively decreases the Debye length of the electric double layer and stabilizes the van der Waals forces of the constituting components, leading to superstruc-ture formation while preventing fusion between individual nanosheets (Figure 4 b). [ 19 ] Following this step, several series of stacked VO 2 (B) nanosheets will coalesce together to form the star-like architecture through the oriented attachment mechanism, as depicted in Figure 4 c. [ 36 ] There may be some degree of subsequent coarsening after the process is com-plete, but fusion of the individual VO 2 (B) nanosheets should be circumvented due to the presence of the oxalic acid derived chelating agent.
Figure 5 presents the cyclic voltammetry (CV), variable rate discharge, cyclic stability curves, and comparison of the
nanosheet surface) while residual chelating agent on the surface prevents fusion; c) series of stacked VO 2 (B) nanosheets then form the star-like architecture through the oriented attachment mechanism. along a crystallographic register; a SAED pattern for a mesocrystal is nearly identical to that of a single crystal-line sample of the same material, making SAED a pop-ular method for characterizing mesocrystals. Figure 3 c displays the corresponding SAED pattern of the region from Figure 3 b. The single crystal-like diffraction pattern is consistent with literature reports that index similar pat-terns as single crystalline VO 2 (B).
[ 3032 ] Some distortion of the SAED pattern should be expected as the TEM image clearly shows that there are secondary particles present in addition to the arms of the cross sectioned star-structure being examined.
Figure 3 d displays a magnifi ed TEM image of a VO 2 (B) star-assembly edge. The single crystalline nature of the VO 2 (B) nanosheet is clearly visible as noted by the lattice fringes, and the dispersion of pores throughout the struc-ture is also apparent. The preferred growth direction of the VO 2 (B) structure is realized by considering the rela-tive stacking rate of the octahedra at various crystal faces (Figure S1, Supporting Information). The shortest average bond in the VO 2 (B) structure is along the  direction, which, based on the proposed formation mechanism, can account for the shape of the synthesized nanosheets and the o...